Y. Hu · J. Gu · F. Wang

College of Material Science and Engineering, Northeast Forestry University, Harbin 150040, China

T. Nakao (*) · T. Nakai

Faculty of Science and Engineering, Shimane University, Matsue 690-8504, Japan

Tel. 81-852-32-6564; Fax 81-852-32-6123 e-mail: nakaote@riko.shimane-u.ac.jp

Received: July 18, 2003 / Accepted: December 15, 2003

**Abstract Wood plastic plywood (WPPW), composed of**
veneer and styrofoam, was manufactured without special
adhesives such as urea–formaldehyde or
phenol–formalde-hyde resins, and its vibrational properties were investigated.
WPPW can be produced at 1 MPa and 160°C for 9 min
(three-ply) and 12 min (five-ply). The dynamic Young’s
modulus reached its highest value when the styrofoam
thickness was 30 mm. The sound velocity and dynamic
Young’s modulus had minimum values at a grain angle of
45°. The results for dynamic Young’s moduli measured by a
longitudinal vibration method and an in-plane flexural
vibration method were almost the same. Dynamic shear
moduli were measured by an in-plane surface wave
propa-gation test and an in-plane flexural vibration method. From
the experimental results, the dynamic shear moduli at 0°
and 90° by the two methods were relatively close, although
the surface wave propagation test results were higher than
those from the flexural vibration method. Dynamic shear
moduli at a grain angle of 45° measured by the in-plane
surface wave propagation test and calculated from theory
were relatively close. The surface wave propagation test
results were smaller than the results calculated from theory.
The shear stress distribution factors were about 1.000–1.189
for WPPW.

**Key words Wood plastic plywood · Sound velocity · **
Dy-namic Young’s modulus · DyDy-namic shear modulus ·
Vibra-tion method

### Introduction

Plywood is an important wood-based panel with many ad-vantages. However, formaldehyde released from plywood, especially from urea–formaldehyde bonded plywood, is a pollution problem. Formaldehyde can pollute outdoor and indoor air and is harmful to human health. Formaldehyde in the air irritates the eyes, nose, and throat, and may even contribute to cancer. On the other hand, styrofoam is very useful as a packaging material. However, unless it is prop-erly recycled after use it can become a pollution problem. Wood plastic plywood (WPPW) is made by combining wooden elements and plastic elements (styrofoam). Not only can WPPW decrease pollution caused by styrofoam waste and formaldehyde released from plywood, it is also economical because no special adhesives such as urea– formaldehyde resins or phenol–formaldehyde resins are re-quired. In our study, wood plastic plywood (WPPW) composed of veneer and styrofoam was manufactured, and its vibrational properties were investigated.

The sound velocity, Young’s modulus, and shear modu-lus are important properties for wood and wood-based panel products. The Young’s modulus and shear modulus can be used to predict bending strengh.1

In this article, the effects of the grain angles of face veneer on sound velocities and dynamic Young’s moduli of WPPW are discussed. The effect of styrofoam thickness on dynamic Young’s modulus of WPPW was also investigated. Various testing methods are available to determine the shear modulus, however, there exists a considerable difference between the shear modulus values determined by each method. Furthermore, these tests have their drawbacks.2–4

### Materials and methods

MaterialsThe experimental panels were made from wood and plastic
*elements. As shown in Fig. 1, lauan (Shorea spp.) veneer*
(density: 0.455 g/cm3

, thickness: 3.5 mm) was chosen as the wood (W) element. Styrofoam (density: 0.013 g/cm3

, thick-ness: 10, 20, 30, 40, and 50 mm) was chosen as the plastic (P) element.

Panel manufacturing

All experimental panels (600 600 mm) were fabricated in the laboratory. There was no adhesive between the wood and plastic elements. The wood–plastic plywoods were hot-pressed at 1 MPa and 160°C for 9 min (three-ply) and 12 min (five-ply). Specimen size was 300 50 mm.

Vibration method

*Longitudinal transmission method*

The longitudinal transmission method is shown in Fig. 2. The sound transmission time propagating through the specimen was measured with a fast Fourier transform (FFT) analyzer.

The sound velocity and dynamic Young’s modulus were calculated based on Eqs. 1 and 2:5

*V* *L T* (1)

*E* r*V*2 _{(2)}

*where V is sound velocity, L is length of the specimen, T is*
*transmission time, E is dynamic Young’s modulus, and *r is
density of the specimen.

*Longitudinal vibration method*

The specimen was lightly supported in a horizontal
orienta-tion by the fingers at the center of the specimen while they
were tapped by a small hammer at the end of the specimen.
The tap tone was detected by a microphone at the other end
of the beam. The resonance frequencies of the tap tone
were identified by the FFT analyzer. The Young’s modulus
*of free–free longitudinal vibration (Ep) was calculated using*
the following equation:

*E* *Lf*

*n* *n*

*p*

*n*

r 2 1 2

2

Ê Ë

Á ˆ

¯

˜ , , 3, . . . (3)

**Fig. 1. Construction of WPPW before hot pressing for a three-ply and b five-ply**

**Fig. 2. Longitudinal transmission method. FFT, fast Fourier transform****a**

vibration system. The vibrating frequency was detected by a
high-sensitivity microphone connected to an amplifier and a
FFT analyzer. The resonant frequencies of the first, second,
and third nodes were obtained by giving a blow to an edge
of the beam and recording the results with the FFT
ana-lyzer. In this study, in-plane vibration tests were carried out.
*The dynamic in-plane Young’s modulus (Ef) and the ratio*
of dynamic shear modulus and shear stress distribution
*fac-tor (G/*k*f*) were obtained from the TGH flexural vibration
method, including the influence of shear and rotatory
inertia.6

*Surface wave propagation test*

As shown in Fig. 3, the acceleration pickups were glued to
the specimen with adhesive. The specimen was supported at
the nodal points by the foamed styrene. One side of the
specimen was struck with a small wood bar. The time
differ-ence of the wave arriving at the two acceleration pickups on
the specimen was measured by the FFT analyzer. The
*dy-namic shear modulus (G/*k*v) was calculated using the *
fol-lowing equation:

*G*k*v* r*V* *V* *L T*

2

, (4)

where r* is density of the specimen, V is surface wave *
*propa-gation velocity, L is length between the two acceleration*
*pickups, T is surface wave propagation time, and *k*v is shear*
stress distribution factor.

The measurements were carried out in a room main-tained at 20°C and 65% relative humidity.

### Results and discussion

Sound velocityThe effect of grain angle of face veneer on sound velocity of WPPW is shown in Fig. 4. It is obvious from Fig. 4, in WPPW (styrofoam thickness before hot press was 10 mm), the sound velocity decreased with increases of grain angle from 0° to 45°. The sound velocity of WPPW with a face veneer grain angle of 0° was approximately twice that of WPPW with a face veneer grain angle of 45°. On the other hand, the sound velocity increased with increasing grain angle from 45° to 90°. Sound velocity in WPPW with a face veneer grain angle of 45° was approximately 60% of that of WPPW with a face veneer grain angle of 90°.

Dynamic Young’s modulus

The effect of styrofoam thickness on the dynamic Young’s modulus of WPPW by longitudinal transmission method is shown in Fig. 5. The result shows that the dynamic Young’s modulus increased with increases of styrofoam thickness of 10 mm to 30 mm. However, in the range of 30–50 mm, the dynamic Young’s modulus gradually decreased with in-creasing styrofoam thickness. The dynamic Young’s modu-lus reached its largest value when styrofoam thickness was 30 mm.

**Fig. 4. Effect of grain angle (***θ) of face veneer on sound velocity (V) of*
WPPW

The results of measuring dynamic Young’s moduli of WPPW (styrofoam thickness before hot press was 10 mm) by the longitudinal vibration method and in-plane flexural vibration method are shown in Tables 1 and 2. The dynamic Young’s moduli for three-ply WPPW with a face veneer grain angle of 0° were approximately seven times higher than those of WPPW with a face veneer grain angle of 45°, and approximately twice those of WPPW with a face veneer grain angle of 90°. The dynamic Young’s moduli for five-ply WPPW with a face veneer grain angle of 0° were approxi-mately six times higher than those of WPPW with a face veneer grain angle of 45°, and approximately 1.6 times higher than those of WPPW with a face veneer grain angle of 90°. This result was similar to that for conventional ply-wood.7

In addition, it is obvious from Tables 1 and 2 that the dynamic Young’s moduli of WPPW measured by longitudi-nal vibration and in-plane flexural vibration methods were almost the same. This result is similar to that of others.8

Dynamic shear modulus

The results of dynamic shear moduli of WPPW (styrofoam thickness before hot press was 10 mm) by surface wave propagation and flexural vibration methods are shown in Table 3. For WPPW, in-plane dynamic shear moduli at

grain angles of 0° and 90° measured by the two methods were relatively close. However, the surface wave propaga-tion test results were greater than those from the flexural vibration tests.

To verify the validity of in-plane dynamic shear moduli for the face veneer grain angle of 45° by a surface wave propagation test, the following equations were examined:9,10

1 1

2 1 1 2 2

2 2

*Gθ* *G* *θ* *E* *E* *E*

*γ* _{θ}

LT L T

LT

T

cos Ê sin

Ë

Á ˆ

¯

˜ (5)

1 1 4 1 4 1 2 2 2

*E _{θ}*

*E*

*θ*

*E*

*θ*

*G*

*E*

*γ* _{θ}_{θ}

L T LT

LT

L

cos sin Ê sin cos

Ë

Á ˆ

¯ ˜

(6)
where *θ is the grain angle of face veneer of the specimen, Gθ*

*is the shear modulus, Eθ is the Young’s modulus, EL and ET*

*are the Young’s moduli in the L and T directions, GLT is the*
shear modulus in the LT plane, and *γ*LT is Poisson’s ratio in
the LT plane.

When *θ* 45°, Eq. 5 can be represented as follows:

1 1 1 2

45

*G* *E*L *E*T *E*

LT

T

*γ*

(7)

When *θ* 45°, Eq. 6 can be represented as follows:
**Table 1. Dynamic Young’s modulus of wood plastic plywood (WPPW) by longitudinal vibration**

method

Types of WPPW Density (g/cm3_{)} _{E}

0 (GPa) *E*45 (GPa) *E*90 (GPa) *E*0*/E*45 *E*0*/E*90

Three-ply WPPW 0.536 7.760 1.127 3.899 6.886 1.990

Five-ply WPPW 0.553 7.935 1.324 4.966 5.993 1.598

*E*0*, Dynamic Young’s modulus in the face veneer grain angle of 0°; E*45, dynamic Young’s modulus

*in the face veneer grain angle of 45°; E*90, dynamic Young’s modulus in the face veneer grain angle

of 90°

**Table 2. Dynamic Young’s modulus of WPPW by in-plane flexural vibration method**

Types of WPPW Density (g/cm3_{)} _{E}

0 (GPa) *E*90 (GPa) *E*0*/E*90

Three-ply WPPW 0.536 7.614 3.944 1.931

Five-ply WPPW 0.553 7.772 4.856 1.600

**Table 3. Comparison of in-plane dynamic shear modulus of WPPW by two methods**

Types of WPPW *θ *(°) *Gf (GPa)* *Gcp (GPa)* *Gv (GPa)* *Gv/Gf* k*v* (45°) k*v* (0°, 90°)

Three-ply WPPW 0 0.291 – 0.315 1.082 – 1.109

45 – 1.520 1.392 – 1.092 –

90 0.289 – 0.339 1.173 – 1.023

Five-ply WPPW 0 0.359 – 0.402 1.120 – 1.072

45 – 2.386 2.007 – 1.189 –

90 0.353 – 0.381 1.079 – 1.112

angle of 45° measured by the in-plane surface wave propa-gation test and calculated by Eq. 9 were relatively close. However, the surface wave propagation test results were lower than the results calculated by Eq. 9.

Shear stress distribution factor

According to the report by Hearmon,11 the following equa-tion is given:

1_{ } 3_{ }1 2 2_{ }2 _{ }2 0

*d q* *e* *f q* *f f* *q* *f*

### (

### )

### (

### )

### (

### )

(10)where
*q*
*c* *d*
*c*
*c* *e*
*c*
*c* *f*
*c*
*c*
*c*
*c c*
1
66
66
22
11
22
11
66
12
2
22 66
, , ,
and
*c* *c*
*c* *c*
*c*
*E* *E*
*E* *E*
*G*
11 12
21 22
66
1
È
Î
Í
Í
Í
˘
˚
˙
˙
˙
È
Î
Í
Í
Í
Í
Í
Í
Í
˘
˚
˙
˙
˙
˙
˙
˙
˙
L
LT
L
LT
L T
LT
1
1
*γ*
*γ*

*To surface wave propagation, q can be represented as*
follows (0° and 90° grain angle WPPW):

*q*

*v*
1

k (11)

In general, Eq. 10 has one real root. Therefore, the shear
stress distribution factor k*v can be calculated. For three-ply*
WPPW, k*v 1.001. For five-ply WPPW, *k*v 1.000.*

Table 3 and the above analysis show that k*v * 1.000–
1.189 for WPPW.

### Conclusions

The vibrational properties of WPPW were discussed. The following conclusions have been drawn. The sound velocity

thickness was 30 mm.

Dynamic shear moduli were measured by an in-plane surface wave propagation test and an in-plane flexural vi-bration method. From experimental results, the dynamic shear moduli at 0° and 90° by the two methods were rela-tively close. The surface wave propagation test results were greater than those from the flexural vibration method. Dy-namic shear moduli a grain angle of 45° measured by the in-plane surface wave propagation test and calculated from theory were relatively close. The surface wave propagation test results were smaller than those calculated by theory. The shear stress distribution factors were about 1.000–1.189 for WPPW.

### References

1. Chui YH, Smith I (1991) The use of bending and shear moduli for predicting bending strength of wood. Forest Prod J 41:49–52 2. Nakao T, Okano T (1987) Evaluation of modulus of rigidity by

dynamic plate shear testing. Wood Fiber Sci 19:332–338

3. Yoshihara H, Kubojima Y (2002) Measurement of the shear modu-lus of wood by asymmetric four-point bending tests. J Wood Sci 48:14–19

4. van Wyk WJ, Gerischer GFR (1988) A method for determining the G-modulus of wood. Holzforschung 42:191–194

5. Mishiro A (1996) Effects of grain and ring angles on ultrasonic velocity in wood. Mokuzai Gakkaishi 42:211–215

6. Hearmon RFS (1958) The influence of shear and rotatory inertia on the free flexural vibration of wooden beams. Br J Appl Phys 9:381–388

7. Sobue N (1982) Dynamic viscoelasticity of wood-based panel (in Japanese). Wood Ind 37:25–28

8. Dong Y, Nakao T, Tanaka C, Takahashi A, Nishino Y (1994) Dynamic properties of laterally inhomogeneous wood-based pan-els by flexural and longitudinal vibrations (in Japanese). Mokuzai Gakkaishi 40:1302–1309

9. Hayashi T (1971) Composite material engineering (in Japanese). Nikkagiren, Tokyo, Japan

10. Hearmon RFS (1948) Elasticity of wood and plywood. Forest Prod Res Special Report No.7, London